Awarded as the best online publication by CIDC
AGGREGATE IMPACT VALUE
This test is done to determine the aggregate impact value of coarse aggregates as per IS: 2386 (Part IV) – 1963. The apparatus used for determining aggregate impact value of coarse aggregates is
Impact testing machine conforming to IS: 2386 (Part IV)- 1963,IS Sieves of sizes – 12.5mm, 10mm and 2.36mm, A cylindrical metal measure of 75mm dia. and 50mm depth, A tamping rod of 10mm circular cross section and 230mm length, rounded at one end and Oven.
Preparation of Sample
i) The test sample should conform to the following grading:
– Passing through 12.5mm IS Sieve – 100%
– Retention on 10mm IS Sieve – 100%
ii) The sample should be oven-dried for 4hrs. at a temperature of 100 to 110oC and cooled.
iii) The measure should be about one-third full with the prepared aggregates and tamped with 25 strokes of the tamping rod.
A further similar quantity of aggregates should be added and a further tamping of 25 strokes given. The measure should finally be filled to overflow, tamped 25 times and the surplus aggregates struck off, using a tamping rod as a straight edge. The net weight of the aggregates in the measure should be determined to the nearest gram (Weight ‘A’).
Procedure to determine Aggregate Impact Value
i) The cup of the impact testing machine should be fixed firmly in position on the base of the machine and the whole of the test sample placed in it and compacted by 25 strokes of the tamping rod.
ii) The hammer should be raised to 380mm above the upper surface of the aggregates in the cup and allowed to fall freely onto the aggregates. The test sample should be subjected to a total of 15 such blows, each being delivered at an interval of not less than one second.
ii) The ratio of the weight of the fines formed to the total sample weight should be expressed as a percentage.
Aggregate impact value = (B/A) x 100%
iii) Two such tests should be carried out and the mean of the results should be reported.